# Ti-6Al-4V

Last updated

Ti-6Al-4V (UNS designation R56400), also sometimes called TC4, Ti64, [1] or ASTM Grade 5, is an alpha-beta titanium alloy with a high specific strength and excellent corrosion resistance. It is one of the most commonly used titanium alloys and is applied in a wide range of applications where low density and excellent corrosion resistance are necessary such as e.g. aerospace industry and biomechanical applications (implants and prostheses).

## Contents

Studies of titanium alloys used in armors began in the 1950s at the Watertown Arsenal, which later became a part of the Army Research Laboratory. [2] [3]

Increased use of titanium alloys as biomaterials is occurring due to their lower modulus, superior biocompatibility and enhanced corrosion resistance when compared to more conventional stainless steels and cobalt-based alloys. [4] These attractive properties were a driving force for the early introduction of a (cpTi) and a#b (Ti—6Al—4V) alloys as well as for the more recent development of new Ti-alloy compositions and orthopaedic metastable b titanium alloys. The latter possess enhanced biocompatibility, reduced elastic modulus, and superior strain-controlled and notch fatigue resistance. [5] However, the poor shear strength and wear resistance of titanium alloys have nevertheless limited their biomedical use. Although the wear resistance of b-Ti alloys has shown some improvement when compared to a#b alloys, the ultimate utility of orthopaedic titanium alloys as wear components will require a more complete fundamental understanding of the wear mechanisms involved.

## Chemistry

(in wt. %) [6]

V Al Fe O C N H Y Ti Remainder EachRemainder Total
Min3.55.5------------------
Max4.56.75.3.2.08.05.015.005Balance.1.3

## Physical and Mechanical Properties

Ti-6Al-4V titanium alloy commonly exists in alpha, with hcp crystal structure, (SG : P63/mmc) and beta, with bcc crystal structure, (SG : Im-3m) phases. While mechanical properties are a function of the heat treatment condition of the alloy and can vary based upon properties, typical property ranges for well-processed Ti-6Al-4V are shown below. [7] [8] [9] Aluminum stabilizes the alpha phase, while vanadium stabilizes the beta phase. [10] [11]

Density, g/cm3Young's Modulus, GPaShear Modulus, GPaBulk Modulus,GPaPoisson's RatioYield Stress, MPa (Tensile)Ultimate Stress, MPa (Tensile)Hardness, Rockwell CUniform Elongation, %
Min4.4291044096.80.3188090036 (Typical)5
Max4.512113451530.37920950--18

Ti-6Al-4V has a very low thermal conductivity at room temperature, 6.7 - 7.5 W/m·K, [12] [13] which contributes to its relatively poor machinability. [13]

The alloy is vulnerable to cold dwell fatigue. [14]

## Heat Treatment of Ti-6Al-4V

Ti-6Al-4V is heat treated to vary the amounts of and microstructure of ${\displaystyle \alpha }$ and ${\displaystyle \beta }$ phases in the alloy. The microstructure will vary significantly depending on the exact heat treatment and method of processing. Three common heat treatment processes are mill annealing, duplex annealing, and solution treating and aging. [15]

## Applications

• Implants and prostheses (wrought, cast or by Additive Manufacturing (AM)) [16]
• Additive Manufacturing [17]
• Parts and prototypes for racing and aerospace industry. Used extensively within the Boeing 787 aircraft.
• Marine applications
• Chemical industry
• Gas turbines
• Firearm Silencers

## Specifications

• UNS: R56400
• AMS Standard: 4911
• ASTM Standard: F1472
• ASTM Standard: B265 Grade 5 [18]

## Related Research Articles

Stainless steel is a group of ferrous alloys that contain a minimum of approximately 11% chromium, a composition that prevents the iron from rusting and also provides heat-resistant properties. Different types of stainless steel include the elements carbon, nitrogen, aluminium, silicon, sulfur, titanium, nickel, copper, selenium, niobium, and molybdenum. Specific types of stainless steel are often designated by their AISI three-digit number, e.g., 304 stainless. The ISO 15510 standard lists the chemical compositions of stainless steels of the specifications in existing ISO, ASTM, EN, JIS, and GB (Chinese) standards in a useful interchange table.

Titanium is a chemical element with the symbol Ti and atomic number 22. Its atomic weight is 47.867 measured in daltons. It is a lustrous transition metal with a silver color, low density, and high strength. Titanium is resistant to corrosion in sea water, aqua regia, and chlorine.

Titanium diboride (TiB2) is an extremely hard ceramic which has excellent heat conductivity, oxidation stability and wear resistance. TiB2 is also a reasonable electrical conductor, so it can be used as a cathode material in aluminium smelting and can be shaped by electrical discharge machining.

In modern Western body piercing, a wide variety of materials are used. Some cannot be autoclaved, and others may induce allergic reactions, or harbour bacteria. Certain countries, such as those belonging to the EU, have legal regulations specifying which materials can be used in new piercings.

Titanium nitride is an extremely hard ceramic material, often used as a coating on titanium alloys, steel, carbide, and aluminium components to improve the substrate's surface properties.

Titanium alloys are alloys that contain a mixture of titanium and other chemical elements. Such alloys have very high tensile strength and toughness. They are light in weight, have extraordinary corrosion resistance and the ability to withstand extreme temperatures. However, the high cost of both raw materials and processing limit their use to military applications, aircraft, spacecraft, bicycles, medical devices, jewelry, highly stressed components such as connecting rods on expensive sports cars and some premium sports equipment and consumer electronics.

Microstructure is the very small scale structure of a material, defined as the structure of a prepared surface of material as revealed by an optical microscope above 25× magnification. The microstructure of a material can strongly influence physical properties such as strength, toughness, ductility, hardness, corrosion resistance, high/low temperature behaviour or wear resistance. These properties in turn govern the application of these materials in industrial practice.

An archwire in orthodontics is a wire conforming to the alveolar or dental arch that can be used with dental braces as a source of force in correcting irregularities in the position of the teeth. An archwire can also be used to maintain existing dental positions; in this case it has a retentive purpose.

The SAE steel grades system is a standard alloy numbering system for steel grades maintained by SAE International.

Aluminium alloys are alloys in which aluminium (Al) is the predominant metal. The typical alloying elements are copper, magnesium, manganese, silicon, tin and zinc. There are two principal classifications, namely casting alloys and wrought alloys, both of which are further subdivided into the categories heat-treatable and non-heat-treatable. About 85% of aluminium is used for wrought products, for example rolled plate, foils and extrusions. Cast aluminium alloys yield cost-effective products due to the low melting point, although they generally have lower tensile strengths than wrought alloys. The most important cast aluminium alloy system is Al–Si, where the high levels of silicon (4.0–13%) contribute to give good casting characteristics. Aluminium alloys are widely used in engineering structures and components where light weight or corrosion resistance is required.

6061 is a precipitation-hardened aluminium alloy, containing magnesium and silicon as its major alloying elements. Originally called "Alloy 61S", it was developed in 1935. It has good mechanical properties, exhibits good weldability, and is very commonly extruded. It is one of the most common alloys of aluminum for general-purpose use.

7075 aluminium alloy (AA7075) is an aluminium alloy, with zinc as the primary alloying element. It has excellent mechanical properties and exhibits good ductility, high strength, toughness, and good resistance to fatigue. It is more susceptible to embrittlement than many other aluminium alloys because of microsegregation, but has significantly better corrosion resistance than the alloys from the 2000 series. It is one of the most commonly used aluminium alloys for highly stressed structural applications and has been extensively used in aircraft structural parts.

Nitinol biocompatibility is an important factor in biomedical applications. Nitinol (NiTi), which is formed by alloying nickel and titanium, is a shape memory alloy with superelastic properties more similar to that of bone, when compared to stainless steel, another commonly used biomaterial. Biomedical applications that utilize Nitinol include stents, heart valve tools, bone anchors, staples, septal defect devices and implants. It is a commonly used biomaterial especially in the development of stent technology.

Titanium Beta C refers to Ti Beta-C, a trademark for an alloy of titanium originally filed by RTI International. It is a metastable "beta alloy" which was originally developed in the 1960s; Ti-3Al-8V-6Cr-4Mo-4Zr, nominally 3% aluminum, 8% vanadium, 6% chromium, 4% molybdenum, 4% zirconium and balance (75%): titanium.

Cobalt-chrome or cobalt-chromium (CoCr) is a metal alloy of cobalt and chromium. Cobalt-chrome has a very high specific strength and is commonly used in gas turbines, dental implants, and orthopedic implants.

2219 aluminium alloy is an alloy in the wrought aluminium-copper family. It can be heat-treated to produce tempers with higher strength but lower ductility. The aluminium-copper alloys have high strength, but are generally less corrosion resistant and harder to weld than other types of aluminium alloys. To compensate for the lower corrosion resistance, 2219 aluminium can be clad in a commercially pure alloy such as 1050 or painted. This alloy is commonly formed by both extrusion and forging, but is not used in casting.

Ti-6Al-2Sn-4Zr-2Mo, also known as Ti 6-2-4-2, is a near alpha titanium alloy known for its high strength and excellent corrosion resistance. It is often used in the aerospace industry for creating high-temperature jet engines and the automotive industry to create high performance automotive valves.

Inconel Alloy 625 is a nickel-based superalloy that possesses high strength properties and resistance to elevated temperatures. It also demonstrates remarkable protection against corrosion and oxidation. Its ability to withstand high stress and a wide range of temperatures, both in and out of water, as well as being able to resist corrosion while being exposed to highly acidic environments makes it a fitting choice for nuclear and marine applications.

Ti-6Al-7Nb is an alpha-beta titanium alloy first synthesized in 1977 containing 6% aluminum and 7% niobium. It features high strength and has similar properties as the cytotoxic vanadium containing alloy Ti-6Al-4V. Ti-6Al-7Nb is used as a material for hip prostheses.

Aluminium 7050 alloy is a heat treatable alloy. It has high toughness, high strength. It has high stress corrosion cracking resistance. It has electric conductivity of value having 40 percent of copper. 7050 aluminium is known as a commercial aerospace alloy.

## References

1. Paul K. Chu; XinPei Lu (15 July 2013). Low Temperature Plasma Technology: Methods and Applications. CRC Press. p. 455. ISBN   978-1-4665-0991-7.
2. "Founding of ARL". www.arl. army.mil. Army Research Laboratory. Retrieved 6 June 2018.
3. Gooch, William A. "The Design and Application of Titanium Alloys to U.S. Army Platforms -2010" (PDF). U.S. Army Research Laboratory. Retrieved 6 June 2018.
4. Long, M.; Rack, H.J. (1998). "Titanium alloys in total joint replacement—a materials science perspective". Biomaterials. 18 (19): 1621–1639. doi:10.1016/S0142-9612(97)00146-4. PMID   9839998.
5. Gutmanas, E.Y.; Gotman, I. (2004). "PIRAC Ti nitride coated Ti–6Al–4V head against UHMWPE acetabular cup–hip wear simulator study". Journal of Materials Science: Materials in Medicine. 15 (4): 327–330. doi:10.1023/B:JMSM.0000021096.77850.c5. PMID   15332594. S2CID   45437647.
6. "Titanium Ti-6Al-4V (Grade 5), Annealed". asm.matweb.com. ASM Aerospace Specification Metals, Inc. Retrieved 14 March 2017.
7. "Titanium Alloy Ti 6Al-4V Technical Data Sheet". cartech.com. Carpenter Technology Corporation. Retrieved 14 March 2017.
8. "AZoM Become a Member Search... Search Menu Properties This article has property data, click to view Titanium Alloys - Ti6Al4V Grade 5". www.azom.com. AZO Materials. Retrieved 14 March 2017.
9. Wanhill, Russell; Barter, Simon (2012), "Metallurgy and Microstructure", Fatigue of Beta Processed and Beta Heat-treated Titanium Alloys, Springer Netherlands, pp. 5–10, doi:10.1007/978-94-007-2524-9_2, ISBN   9789400725232
10. Donachie, Matthew J. (2000). (2nd ed.). Materials Park, OH: ASM International. pp.  13–15. ISBN   9781615030620. OCLC   713840154.
11. "ASM Material Data Sheet". asm.matweb.com. Retrieved 2020-06-20.
12. Yang, Xiaoping; Liu, C. Richard (1999-01-01). "Machining Titanium and Its Alloys". Machining Science and Technology. 3 (1): 107–139. doi:10.1080/10940349908945686. ISSN   1091-0344.
13. BEA (September 2020). "AF066 crash investigation results" (PDF).
14. ASM Committee (2000). "The Metallurgy of Titanium". Titanium: A Technical Guide. ASM International. pp. 22–23.
15. "Ti6Al4V Titanium Alloy" (PDF). Arcam.
16. "Ti64 Titanium Alloy Powder". Tekna.
17. "§1.1.5", ASTM B265-20a, Standard Specification for Titanium and Titanium Alloy Strip, Sheet, and Plate, West Conshohocken, PA: ASTM International, 2020, doi:10.1520/B0265-20A , retrieved 13 August 2020